tissue engineering of injectable soft tissue filler: using ... engineering of injectable soft tissue...
Embed Size (px)
A number of injectable materials have popularly been usedto treat soft tissue defects, although fat injections or grafts aremost popular. Micronized acellular dermal matrix (Alloderm),an injectable material, is a highly versatile intermediate-lengthimplant with many applications. However, though cell in-growths and revascularization of implanted micronized Allo-derm are an important factor for lasting the length of results,this process unfortunately does not appear to occur in every-one (1). To improve results after injecting micronized Allo-derm, the authors admixed micronized Alloderm with adi-pose stem cells (ASCs). ASCs have been used in adipose tis-sue engineering (2, 3), because ASCs, harvested sufficientlyfrom adipose tissue, are known to possess the ability of highproliferation and strong differentiation to adipocytes (4) andendothelial cells (5). The authors considered that adipocytesdifferentiated from ASCs in micronized Alloderm wouldmake the injected micronized Alloderm a more acceptablesoft tissue substitute, and the differentiated endothelial cellswould enhance implantation of the injected soft tissue con-structs.
To develop an injectable soft tissue filler, the authors triedto produce adipose tissue equivalents using ASCs and micro-
nized Alloderm as scaffold by introducing the concept oftissue engineering.
MATERIALS AND METHODS
Isolation and multiplication of human ASCs
Human ASCs were isolated from adipose tissue obtained byabdominoplasty via enzymatic digestion. Briefly, after remov-ing visible fibrous tissue and vessels, adipose tissue was fine-ly minced and enzymatically digested in dulbeccos modifiedeagles medium (DMEM)/F-12 media (Gibco, Gaithersburg,MD, U.S.A.) containing 0.1% type I collagenase (SigmaChemical Co., St. Louis, MO, U.S.A.), 1% fatty acid freebovine serum albumin (Sigma), and 1× Penicillin-Strepto-mycin (Gibco) for 30 min at 37℃ at adipose tissue to a dis-sociation medium ratio of 2 g/1 mL. The digested tissue wasfiltered through cotton gauze, and the filtrate suspensionwas centrifuged at 1,000 rpm for 5 min, cell pellet were thenresuspended in DMEM/F-12 media (Gibco) supplementedwith 10% bovine calf serum (Hyclone, Logan, UT, U.S.A.)and 1× penicillin-streptomycin (Sigma). ASCs were platedat 104 cells/mL and passaged two or three times.
Gyeol Yoo and Jin Soo Lim
Department of Plastic Surgery, the Catholic Universityof Korea, Seoul, Korea
Address for correspondenceJin Soo Lim, M.D.Department of Plastic Surgery, College of Medicine,the Catholic University of Korea, St. Vincent’s Hospital, 93-6 Ji-dong, Paldal-gu, Suwon 442-723,KoreaTel : +82.31-249-7206, Fax : +82.31-241-0005E-mail : [email protected]
J Korean Med Sci 2009; 24: 104-9ISSN 1011-8934DOI: 10.3346/jkms.2009.24.1.104
Copyright � The Korean Academyof Medical Sciences
Tissue Engineering of Injectable Soft tissue Filler: Using AdiposeStem Cells and Micronized Acellular Dermal Matrix
In this study of a developed soft tissue filler, adipose tissue equivalents were con-structed using adipose stem cells (ASCs) and micronized acellular dermal matrix(Alloderm). After labeling cultured human ASCs with fluorescent green protein andattaching them to micronized Alloderm (5××105 cells/1 mg), ASC-Alloderm complex-es were cultured in adipogenic differentiation media for 14 days and then injectedinto the dorsal cranial region of nude male mice. The viabilities of ASCs in micronizedAlloderm were determined at 1, 4, 7, and 14 days, and complexes, which had beencultured for 14 days and implanted in vivo for 2 months, were histologically evaluatedby light, confocal, and scanning electron microscopy. The viabilities representedthat ASCs in micronized Alloderm were alive during the culture period. ASC-Allo-derm complexes cultured for 14 days contained round cells with large lipid vesiclesby light microscopy and many spherical cells by SEM. ASCs in implanted ASC-Alloderm complexes harvested from mice at 2 months postinjection were histologi-cally found to have differentiated into adipocytes which had green fluorescencedye. Micronized Alloderm may be found useful as scaffold for human ASCs whenconstructing fat tissue for three-dimensional soft tissue filling. The present studysuggests that ASC-Alloderm complexes can be used as injectable three-dimen-sional soft tissue fillers.
Key Words : Mesenchymal Stem Cells; Alloderm; Tissue Engineering
Received : 16 August 2007Accepted : 29 April 2008
Tissue Engineering of Injectable Soft Tissue Filler 105
Labeling and the induction of differentiation of humanASCs
PKH67 green fluorescent cell linker kits (Sigma) wereused for labeling ASCs. Briefly, ASCs were trypsinized andwashed once with DMEM/F-12 medium without serum. 2×107 cells suspended in medium were placed in 15 mL cen-trifuge tubes, and centrifuged (400× g) for 5 min to formloose pellets. Medium was then carefully aspirated to leaveno more than 25 μL of residual medium on pellets. The cellswere then resuspended in this residual medium, and 1 mLof Diluent C was added. Immediately prior to staining, a 2×staining solution of PKH67 was prepared in polypropylenetube by diluting 4 μL of 1 mM dye stock in 1 mL of Dilu-ent C. Staining was initiated by rapidly adding a 2× con-centrated cell suspension to the 2× dye solution. Stainingwas stopped after 5 min by adding an equal volume (2 mL)of fetal bovine serum over a period of 1 min followed by anequal volume (4 mL) of complete medium containing 10%serum. Cells were then centrifuged and washed three timeswith 10 mL of complete medium. Stained cells were culturedas monolayers in adipogenic differentiation media (Zen-BioCo, Research Triangle, NC, U.S.A.) for 14 days. ASCs cul-tured in adipogenic differentiation media were visualizedand photographed under an inverted microscope (Axiovert200 M, Zeiss, Gottingen, Germany) equipped with a colordigital camera. A fluorescein isothiocyanate fluorescent fil-ter set was used to visualize labeled cells.
In vitro culture and the induction of differentiation of ASC-Alloderm complex
Micronized acellular dermal matrix (micronized Alloderm)was purchased from ShebaTM (Hans Biomed Co., Seoul, Korea).Briefly, micronized Alloderm in a syringe was hydrated with6 mL of DMEM/F-12 media (Gibco) for 30 min, and cen-trifuged at 1,000 rpm for 5 min. Supernatant was aspiratedoff, and 3mL media was added.
ASC-Alloderm complexes were made by mixing humanASCs and micronized Alloderm at 5×104 cells/mg of mic-ronized Alloderm. After incubating with rocking overnight,10 μL aliquots of the complex (10 mg Alloderm with ASCs)were divided into each well of ten 24-well culture plates con-taining 1 mL DMEM/F-12 media supplemented with 10%bovine calf serum, and 100 U/mL penicillin-streptomycin.To induce differentiation, media were replaced with adipo-genic differentiation media 24 hr after plating, and plateswere incubated for 14 days in an incubator (37℃, 5% CO2).Differentiation media were changed every 3 days.
Estimating cell viabilities of ASCs in cultured ASC-Alloderm complexes
At 1, 4, 7, and 14 days after seeding ASCs in micronized
Alloderm, 200 μL of sodium 3′-[1-(phenylamino-carbonyl)-3,4-tetrazolium]-bis (4-methoxy-6-nitro) benzene sulfonicacid hydrate labeling reagent (XTT; Boehringer MannheimGmbH, Mannheim, Germany) with electron-coupling rea-gent were added to each well (described above) and incubat-ed for 24 hr. The absorbances of media in wells were deter-mined at 490 nm and 690 nm by spectrophotometry. Cellviabilities were expressed by calculating the difference bet-ween ‘the defference between two absorbances of media ofsample in well’ and ‘the difference between two absorbancesof DMEM/F-12 medium containing XTT reagent’.
In vivo implantation of ASC-Alloderm complex
Cultured human ASCs were labeled using PKH67 greenfluorescent cell linker kits (Sigma) to determine whether adi-pose formation in complexes originated from seeded cells orfrom surrounding perivascular tissue. Subsequently, ASCswere mixed with micronized Alloderm as described above.ASC-Alloderm complexes were cultured in adipogenic differ-entiation media for 2 weeks, then 50 mg of ASC-Allodermcomplexes were gently injected subcutaneously into the dor-sal cranial region of nude male mice using 1 mL syringe with18 G needle. Among the 8 mice used, 4 mice were injectedwith only micronized Alloderm, and 4 mice were injectedwith ASC-Alloderm complex. Two months later, the fourmice were sacrificed and the injected tissues were excised.The excised masses were weighed and then fixed in 10% for-malin or OCT compound.
ASC-Alloderm complexes were obtained after 14 days ofin vitro culture, and injected tissues were obtained from nudemice 2 months after implantation.
For hematoxylin and eosin (H&E) staining, samples werefixed in 10% formalin, prepared as paraffin blocks, sectionedat 6 μm, and stained with H&E.
For Oil-red O staining, injected ASC-Alloderm complexesexcised from nude mice at 2 months after implantation (frozenin dry ice and stored at -80℃) were placed in a cryomold withOCT (Tissue-Tek�, Sakura Finetek Inc., Torrance, CA, U.S.A.).Ten-micrometer sections were cut using a microtome, placedon slides, and stained with Oil-red O. Nuclei were then coun-terstained with hematoxylin, and sections were then cover-slipped. The slides were examined under a confocal micro-scope (MRC 1024 MP, Bio-Rad, Hercules, CA, U.S.A.).
Scanning electron microscope (SEM)
ASC-Alloderm complexes obtained after 14 days of in vitroculture were treated with a fixative containing 3% glutaralde-hyde and 4% paraformaldehyde in 0.1 M cacodylate buffer(all pH 7.2) for 1 hr at room temperature. Samples were rinsed
106 G. Yoo and J.S. Lim
with 0.1 M cacodylate buffer (3×, 5 min), post-fixed with1% osmium tetroxide in 0.1 M cacodylate buffer for 2 hr,dehydrated in ethanol, subjected to critical point drying,and sputter coated. The samples were examined in a JSM5410 LV (Jeol LTD, Tokyo, Japan) at 5 kV.
Results are expressed as mean±standard deviation. Sta-tistical analysis was performed by one-way analysis of vari-ance (one-way ANOVA) using SPSS Ver. 10 for Windows.Multiple comparison of Scheffe was used for comparing thedifferences for these different culture periods. Differenceswere considered significant at p<0.05.
Monolayer culture of ASCs
After ASCs had been cultured as monolayers in differenti-ation media for 14 days, most were enlarged and containedmany lipid droplets, which were stained by Oil-red O (Fig.1A), showed a green fluorescence (Fig. 1B).
In vitro culture of ASC-Alloderm complex
ASCs viabilities were; 0.61±0.19, 0.71±0.09, 0.79±0.15, and 0.86±0.14 after culture for 1, 4, 7, and 14 days(one-way ANOVA, F=2.939, p=0.065). Although these ratesshowed an increasing tendency with culture time (Fig. 2),
no significant difference was observed for these different cul-ture periods (p>0.05).
By H&E histological examination, some ASCs in mic-ronized Alloderm were observed to have differentiated andto contain large lipid vesicles after 14 days (Fig. 3).
The micronized Alloderm resembled pieces of dried treeroots by SEM (Fig. 4A). After culture for 14 days, many cellswere covered the micronized Alloderm, and some sphericalcells suspected of being adipocytes were observed (Fig. 4B).
In vivo implantation of ASC-Alloderm complex
All animals remained healthy throughout the experimen-
Fig. 1. Microscopic findings of adipose stem cells (ASCs) cultured in a monolayer for 14 days. (A) Some ASCs had differentiated intoadipocytes, which contained many lipid droplets as visualized by Oil-red O staining. (B) ASCs were well labeled with PHK67 green fluo-rescent dye (×400).
0.01 day 4 day 7 day 14 day
Fig. 2. Changes in ASCs viabilities over 14 days in culture. ASCswere cultured in vitro after mixing then with micronized Alloderm(5×104 cells/1 mg of Alloderm). Cell viabilities were determinedusing XTT colorimetric assays. Values represent mean±stan-dard deviation (error bar).
Tissue Engineering of Injectable Soft Tissue Filler 107
tal period. At two months after implantation, injected tis-sues were easily identified in the cranial region. The weightof injected tissues of micronized Alloderm injected groupand ASC-Alloderm complex injected group was 51.4±5.8mg and 54.6±3.7 mg, respectively, but there was no sig-nificant difference between the weights of two groups (p>0.05). An H&E histological examination revealed that somecells and small capillary had infiltrated the micronized der-mal matrix in controls (Fig. 5A), whereas markedly increased
numbers of large signet-ring cells and large capillaries wereobserved in ASC-Alloderm complex injected mice (Fig. 5B).Moreover, in injected ASC-Alloderm complexes, signet-ringcells were stained with Oil-red O and some cells showed weakgreen fluorescent under the confocal microscope (Fig. 6).
Soft tissue defects range from the furrow of rhytid to a majorloss of subcutaneous tissue secondary to congenital malforma-tion, trauma, or extirpation. The reconstruction of such de-fects is the province of plastic surgery. Over the years, variousmethods of fat injection or graft have been used, and variousmaterials evolved to treat such defects. However, these treat-ment have many limitations, such as donor-site morbidityand deformity, unsatisfactory and unpredictable results, andcomplications resulting from the toxicity of implants (6).For abrogating these limitations, adipose tissue engineeringrecently has been proposed as an alternative for currenttreatment (7). The choice of the types of seeding cells andscaffold used in tissue engineering determines the success ofadipose tissue engineering (7).
The adipose stem cells (ASCs) may be an ideal autologouscell source for adipose tissue engineering (8). ASCs are muchmore resistant to mechanical damage and ischemic conditionsthan mature adipocytes (9). Moreover, ASCs can be readilyharvested from excised human subcutaneous fat or liposuc-tion samples, and proliferate rapidly and differentiate intomature adipocytes both in vitro and in vivo (4, 10, 11). Manystudies have recently done using ASCs in adipose tissue engi-neering because ASCs have been demonstrated as a good cell
Fig. 4. Scanning microscopic findings after 14 day of in vitro culture. (A) Micronized Alloderm alone. (B) ASC-Alloderm complex. Manycells were found to cover the micronized Alloderm, and some spherical adipocyte-like cells were observed.
A B400×5 kV 400×5 kV
10 μ 10 μ
Fig. 3. Microscopic findings of in vitro cultured ASC-Alloderm com-plex for 14 days. ASCs in micronized Alloderm differentiated toround cells (arrows) with large lipid vesicles (H&E stain, ×400).
108 G. Yoo and J.S. Lim
source for adipose tissue engineering because of their highproliferation, strong differentiation, and less invasive pro-curement (2, 3). In the present study, as in previous studies,human ASCs were found to differentiate readily to adipocytesin monolayer (2-dimensional culture), in 3-dimensional invitro cultures, and in vivo.
Alloderm has been used as a good scaffold for skin and oralmucosa in tissue engineering, and it has been reported to orga-nize the arrangement of seeded keratinocytes and culturedkeratinocyte sheets into three-dimensional epidermal struc-ture that has several layers, and to recreate the original reteridges at the interface of the dermis (12). The Alloderm hasbeen found to produce composite oral mucosa equivalent con-sisting of a stratified epidermis on a dermal matrix using cul-tured oral keratinocytes and Alloderm (13, 14). In the presentstudy, micronized Alloderm was used as a scaffold of ASCsfor adipose tissue engineering. In the previous study, a num-ber of different scaffolds have been investigated for adiposetissue engineering applications, e.g., polyglycolic acid (PGA)(10), poly (lactic-co-glycolic acid) (PLGA) (15), and hyaluron-ic acid (16). In addition, injectable materials, such as, fibrin(17), matrigel (18), and alginate gel (19) have also been stud-ied as scaffolds for adipose tissue engineering. Injectable scaf-folds can widen the scope of the engineered adipose tissue.This injectable engineered adipose tissue would be easily use-ful in softening wrinkles, augmenting depressed scars, andreconstructing nipples. As micronized Alloderm have beenused for soft tissue augmentation of facial rhytids, scars, anddeformities in injectable form (20), micronized Alloderm hassucceeded to this characteristic when they would be used asa scaffold for adipose tissue engineering. In the present study,XTT cell viability testing showed that ASCs remained viablein micronized Alloderm in vitro. Moreover, these adopted around morphology and contained large lipid vesicles after 14days in culture, which suggests that micronized Alloderm is asuitable ASCs scaffold for adipose tissue engineering purposes.
Fig. 5. Microscopic findings after 2 months of in vivo implantation. (A) Micronized Alloderm alone. Some fibroblast-like cells and few smallcapillaries were observed in the micronized Alloderm. (B) ASC-Alloderm complex. Many signet-ring cells and large capillaries werefound (H&E stain, ×400).
Fig. 6. Confocal microscopic findings of injected ASC-Allodermcomplexes excised at 2 months after implantation. Many signet-ringcells were stained by Oil-red O and some cells showed weak greenfluorescence (Oil-red O stain, ×400).
Tissue Engineering of Injectable Soft Tissue Filler 109
ASC-Alloderm complexes after 2 months in vivo containedmany signet-ring cells and large capillaries, whereas mic-ronized Alloderm alone contained some fibroblast-like cellsand few small capillaries. Moreover, many signet-ring cellsin ASC-Alloderm complexes were stained positively by Oil-red O and also showed green fluorescence indicating thatthe observed differentiated adipocytes originated from inject-ed ASC-Alloderm rather than surrounding fibrovascular tis-sues. Moreover, implanted ASC-Alloderm complex is softerthan micronized Alloderm alone because of this adipose tis-sue development.
In conclusion, the present study suggests that micronizedAlloderm provides a suitable scaffold for ASCs for adiposetissue engineering purpose, and that ASC-Alloderm complexhas potential as a softer, more natural injectable soft tissuefiller.
1. Maloney BP, Murphy BA, Cole HP 3rd. Cymetra. Facial Plast Surg2004; 20: 129-34.
2. Rodriguez AM, Elabd C, Delteil F, Astier J, Vernochet C, Saint-MarcP, Guesnet J, Guezennec A, Amri EZ, Dani C, Ailhaud G. Adipocytedifferentiation of multipotent cells established from human adiposetissue. Biochem Biophys Res Commun 2004; 315: 255-63.
3. Hong L, Peptan IA, Colpan A, Daw JL. Adipose tissue engineeringby human adipose-derived stromal cells. Cells Tissues Organs 2006;183: 133-40.
4. Zuk PA, Zhu M, Mizuno H, Huang J, Futrell JW, Katz AJ, BenhaimP, Lorenz HP, Hedrick MH. Multilineage cells from human adiposetissue: implications for cell-based therapies. Tissue Eng 2001; 7:211-28.
5. Fraser JK, Wulur I, Alfonso Z, Hedrick MH. Fat tissue: an under-appreciated source of stem cells for biotechnology. Trends Biotech-nol 2006; 24: 150-4.
6. Billings E Jr, May JW Jr. Historical review and present status of freefat graft autotransplantation in plastic and reconstructive surgery.Plast Reconstr Surg 1989; 83: 368-81.
7. Patrick CW Jr. Tissue engineering strategies for adipose tissue repair.Anat Rec 2001; 263: 361-6.
8. De Ugarte DA, Ashjian PH, Elbarbary A, Hedrick MH. Future offat as raw material for tissue regeneration. Ann Plast Surg 2003;
50: 215-9.9. von Heimburg D, Hemmrich K, Zachariah S, Staiger H, Pallua N.
Oxygen consumption in undifferentiated versus differentiated adi-pogenic mesenchymal precursor cells. Respir Physiol Neurobiol2005; 146: 107-16.
10. Cho SW, Kim SS, Rhie JW, Cho HM, Choi CY, Kim BS. Engineer-ing of volume-stable adipose tissues. Biomaterials 2005; 26: 3577-85.
11. Zuk PA, Zhu M, Ashjian P, De Ugarte DA, Huang JI, Mizuno H,Alfonso ZC, Fraser JK, Benhaim P, Hedrick MH. Human adiposetissue is a source of multipotent stem cells. Mol Biol Cell 2002; 13:4279-95.
12. Hickerson WL, Compton C, Fletchall S, Smith LR. Cultured epi-dermal autografts and allodermis combination for permanent burnwound coverage. Burns 1994; 20 (Suppl 1): S52-5.
13. Izumi K, Takacs G, Terashi H, Feinberg SE. Ex vivo developmentof a composite human oral mucosal equivalent. J Oral MaxillofacSurg 1999; 57: 571-7.
14. Izumi K, Terashi H, Marcelo CL, Feinberg SE. Development andcharacterization of a tissue-engineered human oral mucosa equiva-lent produced in a serum-free culture system. J Dent Res 2000; 79:798-805.
15. Patrick CW Jr, Chauvin PB, Hobley J, Reece GP. Preadipocyte seed-ed PLGA scaffolds for adipose tissue engineering. Tissue Eng 1999;5: 139-51.
16. Halbleib M, Skurk T, de Luca C, von Heimburg D, Hauner H. Tis-sue engineering of white adipose tissue using hyaluronic acid-basedscaffolds. I: in vitro differentiation of human adipocyte precursorcells on scaffolds. Biomaterials 2003; 24: 3125-32.
17. Schoeller T, Lille S, Wechselberger G, Otto A, Mowlavi A, Piza-Katzer H, Mowlawi A. Histomorphologic and volumetric analysisof implanted autologous preadipocyte cultures suspended in fibringlue: a potential new source for tissue augmentation. Aesthetic PlastSurg 2001; 25: 57-63.
18. Kawaguchi N, Toriyama K, Nicodemou-Lena E, Inou K, Torii S,Kitagawa Y. De novo adipogenesis in mice at the site of injection ofbasement membrane and basic fibroblast growth factor. Proc NatlAcad Sci USA 1998; 95: 1062-6.
19. Yoo G, Yea BH, Rhie JW, Kwon H, Wee SS, Ahn ST. Growth andDifferentiation of Preadipocytes in Alginate and Collagen Gels. JKorean Soc Plast Reconstr Surg 2000; 27: 386-92.
20. Cheng JT, Perkins SW, Hamilton MM. Collagen and injectable fillers.Otolaryngol Clin North Am 2002; 35: 73-85.